PROGRAM I MICRO and NANOFABRICATION - imel. · PDF fileProject Ι. 2: Micro and...
Embed Size (px)
Transcript of PROGRAM I MICRO and NANOFABRICATION - imel. · PDF fileProject Ι. 2: Micro and...
Project . 2: Micro and Nanofabrication using lithography and plasma etching Key researchers: E. Gogolides, A. Tserepi Permanent Researcher: V. Constantoudis Researchers on Contract: G.P. Patsis, G. Kokkoris Collaborating researchers: K. Misiakos, I. Raptis, P. Argitis PhD candidates: M. Vlachopoulou, G. Boulousis, K. Tsougeni, A. Malainou, D. Kontziampasis MSc Students: D. Papageorgiou, K. Ellinas, H. Christoyianni, A. Zeniou, A. Smyrnakis Engineer: A. Zeniou Marie Curie Fellows: Three Marie Curie International Fellows joined our project this year External collaborators: A. Boudouvis and M. Kalantzopooulou (NTUA, Greece), N. Hadjichristidis and E. Iatrou (UoA, Greece), S.Garbis and A. Vlahou (IIBEAA, Greece), S. Kakabakos and P. Petrou (IRRP, NCSR-Demokritos, Greece), G. Kaltsas (TEI Athens Greece), K. Beltsios and I. Panagiotopoulos (U. Ioannina, Greece), E. Gizeli and K. Mitsakakis (Univ. of Crete-FORTH, Greece) C. Cardinaud (U. Nantes, France), I. Rangelow and B. Volland (Univ. Ilmenau Germany), M. Cooke and A. Goodyear (Oxford Instruments Plasma Technology, UK), S. Daniels (DCU, Ireland), A. Erdmann (Fraunhofer, Germany), S. Tedesco, E. Pargon (CEA-LETI, France), A. Speliotis (IMS, NCSR-D)
Projects Running: - EU NMP2 STREP Nanoplasma, Contract No 016424, 1/4/2006-31/3/2009 - GSRT, PENED 03 ED 202, 1/12/2005-30/06/2009 - MD3, IT 214948, 1/12/2007-30/11/2009 - SPAM, Marie Curie-ITN, Contract No 215723
Objectives: Lithography and plasma etching are used as enabling fabrication technologies not only
for traditional sectors, such as electronics and MEMs, but also for microfluidics, microarrays and lab-on-a-chip. We aim in developing deterministic and stochastic microfabrication processes for a broad range of applications including life sciences using top-down fabrication as well as plasma directed assembly: For nano-electronics using e-beam and Double Exposure 193nm lithography, our work
focuses on Line Edge Roughness (LER) prediction using molecular simulation. We have combined our plasma simulation and lithography expertise to predict the LER transfer during plasma etching (see section A).
For microfluidics, we use Deep Plasma Etching to fabricate PDMS, PMMA, PEEK and Si microfluidic devices. We demonstrated smart microfluidics incorporating capillary pumping and hydrophobic valving using our plasma toolbox technology. We also fabricated on chip affinity chromatography columns using TiO2 as stationary phase for phosphopeptide separations (see section B).
In addition using our plasma processes for stochastic nano-texturing of polymers, we demonstrated high density protein microarrays both on PDMS and on PMMA, with almost 10fold higher binding capacity of proteins, and 100fold increased sensitivity compared to flat substrates. We have also optimized novel self aligned processes for protein microarrays on prepatterned substrates (see section B).
We unveiled the mechanisms of plasma nanotexturing and identified the plasma reactor wall as the major factor for nanotexturing. In addition we have devised two methods to produce dual scale roughness on surfaces for control of wetting properties from hydrophilic, to hydrophobic, to oleophobic (see section C). Finally, we have discovered that plasma directed assembly of periodic nanodots can take place during etching of polymers, thus paving the way to plasma based lithography-less nanofabrication.
In order to understand the phenomena of plasma nanotexturing and organization we are also doing Monte Carlo Simulation of plasma surface interactions (see section D).
PPRROOGGRRAAMM II MMIICCRROO aanndd NNAANNOOFFAABBRRIICCAATTIIOONN
RESEARCH RESULTS in 2009: A. Micro & Nanopatterning: Micro and Nano Lithography and Line Edge/ Line Width Roughness (LER, LWR) A1 Molecular simulation of photoresists for double exposure 193nm Lithography (G. P. Patsis, D. Drigiannakis, I. Raptis) Modeling the lithography process with stochastic principles enables the consideration of resist material and process effects variability on critical dimensions and line-edge or line-width roughness of printed features. These principles are applied for a resist system where polymer and photo-acid-generator (PAG) are blended, and for the same system with the PAG molecules bonded on the main polymer chain. Three-dimensional chain-like models of resist and PAG are considered and examples of their effect on critical dimensions and on resist edge roughness were quantified, and compared with experiments from the literature. Fig.1a shows the sample molecules and their digitization scheme in the appropriate format for input to the simulator, while Fig. 1b shows a 3D example of a dissolved resist film.
(b) Fig. 1. (a) Digitization schemes of the molecules used, which are modelled in the current work. (b) 3D simulation results of 32nm resist line of the resist film model. Average CD =32nm. A2 LER transfer during plasma etching (V. Constantoudis, G. Kokkoris, E. Gogolides) The line edge roughness (LER) transfer during plasma etching is theoretically studied. After generating random fractal resist sidewalls with controlled roughness parameters, we model and contrast the nanoscale roughness phenomena for both resist and underlayer sidewalls in a two layer stack using two different plasma processes in three scenarios (Fig. 2a): a) Pattern transfer, b) resist trimming, and c) resist trimming followed by pattern transfer. In the pattern transfer process, etching is considered ion-driven and anisotropic. The protrusions of the rough, trimmed or non-trimmed, resist sidewall act as a shadowing mask for the incident
ions. It is found that shadowing of ions is enough to induce the, well-known by experiments, striations at the sidewalls of both the underlayer and the resist (see Fig. 2b). Pattern transfer induces a decrease of rms roughness but has little effect on the correlation length. In the trimming process, the evolution of the resist sidewall is modelled with an isotropic etching process not affecting the underlayer. The trimming process causes a decrease of the rms value of the resist sidewall and an increase of its correlation length and roughness exponent. In the case of trimming followed by pattern transfer, the striations of the underlayer widen with trimming time and pattern transfer further reduces all LER parameters. The effect of trimming on the rms roughness of the underlayer is important in the case of initially anisotropic resist sidewall.
(a) Before trimming and pattern transfer
(b) After trimming
(c) After trimming and pattern transfer
Ion direction (a) Resist profile before etch (left top). Resist (b) and underlayer (c) after etching (right)
Fig. 2a. The setup of the model and processes. The stack a) after lithography and before (optional) trimming, b) after trimming (isotropic etching) and before pattern transfer, and c) after trimming and pattern transfer (anisotropic etching).
Fig. 2b. The morphology of the resist sidewall after litho (a), and etch (b), and the underlayer sidewall after etch (c)]. The roughness parameters of the initial resist sidewall before trimming (a) are wR,initial=2nm, R,initial=5nm, and R,initial=0.5. Notice the isotropic character of the initial resist surface as well as the anisotropy of the resist and underlayer after pattern transfer.
A3 LER/LWR metrology: Updated version of our software LERDEMO (LERDEMO12) (V. Constantoudis, G.P. Patsis) Fig. 3. The output sheet of the updated version LERDEMO12 with the diagram of the Power Spectrum.
We proceeded to the circulation of a new version of the software LERDEMO developed in our group for LER/ LWR metrology from top-down SEM images taking into account the needs and requests of our client (IMEC, Belgium). The new features added in this version are the following:
1. Calculation of the c-factor, which quantifies the correlations between the edges of a line. This quantity is very useful in double patterning and directed self-assemply techniques, where correlations between the edge fluctuations of a line can be observed.
2. LER/LWR analysis and estimation of LER/LWR parameters for SEM images with anisotropic magnification in which the pixels are asymmetric (rectangular), i.e. x-edge pixel dimension is different than y-dimension.
3. Calculation and presentation in the output sheet of the Power Spectral Density (PSD) of the line widths variation and verification of the Parcevals theorem for the relation between LWR and the area under PSD.
B. Microfluidic and Microarray Fabrication for Life Sciences (see also project III.3) B1 Plasma etching for smart PMMA and PEEK microfluidics with capillary filling and hydrophobic valving (K. Tsougeni, N. Vourdas, D. Papageorgiou, E. Gogolides) We use plasmas for nanotexturing polymeric and silicon surfaces and for selective chemical modification. The combination of both nanotexturing and chemical modification leads to smart surfaces with nice properties such as self-cleaning. The integration of such surfaces in microchannels creates smart microfluidic devices with hydrophilic or hydrophobic patches, which may induce capillary pumping, or superhydrophobic passive valving. Figure 4 shows three types of surfaces in a microchannel with different wetting properties (see the water contact angle on the hydrophobic, superhydrophobic and super hydrophilic stripes in the microchannel inner surface).
Fig. 4. Three types of surfaces in a microchannel with different wetting properties (see the water contact angle on the hydrop